#------------------------------------------------------------------------------
#$Date: 2021-04-12 11:27:20 +0300 (Mon, 12 Apr 2021) $
#$Revision: 264049 $
#$URL: file:///home/coder/svn-repositories/cod/cif/1/56/16/1561653.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_1561653
loop_
_publ_author_name
'Baranets, Sviatoslav'
'Darone, Gregory M.'
'Bobev, Svilen'
_publ_section_title
;
 Synthesis and structure of Sr14Zn1+As11 and Eu14Zn1+As11 (x ≤
 0.5). New members of the family of pnictides isotypic with Ca14AlSb11,
 exhibiting a new type of structural disorder
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              120990
_journal_paper_doi               10.1016/j.jssc.2019.120990
_journal_volume                  280
_journal_year                    2019
_chemical_formula_sum            'As11 Sr14 Zn1.46'
_chemical_formula_weight         2146.32
_space_group_crystal_system      tetragonal
_space_group_IT_number           142
_space_group_name_Hall           '-I 4bd 2c'
_space_group_name_H-M_alt        'I 41/a c d :2'
_atom_sites_solution_hydrogens   .
_atom_sites_solution_primary     dual
_audit_contact_author_name
;
;
_audit_creation_date             2019-08-13
_audit_creation_method
;
Olex2 1.2
(compiled 2018.05.29 svn.r3508 for OlexSys, GUI svn.r5506)
;
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   16.514(4)
_cell_length_b                   16.514(4)
_cell_length_c                   22.366(6)
_cell_measurement_reflns_used    401
_cell_measurement_temperature    200(2)
_cell_measurement_theta_max      19.89
_cell_measurement_theta_min      4.94
_cell_volume                     6099(3)
_computing_cell_refinement       'SAINT V8.38A (?, 2016)'
_computing_data_reduction        'SAINT V8.38A (?, 2016)'
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'ShelXL (Sheldrick, 2015)'
_computing_structure_solution    'ShelXT (Sheldrick, 2015)'
_diffrn_ambient_temperature      200.0
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 1.000
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.2317
_diffrn_reflns_av_unetI/netI     0.1165
_diffrn_reflns_Laue_measured_fraction_full 1.000
_diffrn_reflns_Laue_measured_fraction_max 1.000
_diffrn_reflns_limit_h_max       22
_diffrn_reflns_limit_h_min       -22
_diffrn_reflns_limit_k_max       22
_diffrn_reflns_limit_k_min       -15
_diffrn_reflns_limit_l_max       31
_diffrn_reflns_limit_l_min       -30
_diffrn_reflns_number            25465
_diffrn_reflns_point_group_measured_fraction_full 1.000
_diffrn_reflns_point_group_measured_fraction_max 1.000
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         29.650
_diffrn_reflns_theta_min         2.467
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    37.218
_exptl_absorpt_correction_T_max  0.0387
_exptl_absorpt_correction_T_min  0.0131
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
'SADABS-2016/2 (Bruker,2016/2) was used for absorption correction. wR2(int) was 0.1290 before and 0.0637 after correction. The Ratio of minimum to maximum transmission is 0.3385. The λ/2 correction factor is Not present.'
_exptl_crystal_colour            black
_exptl_crystal_density_diffrn    4.674
_exptl_crystal_description       irregular
_exptl_crystal_F_000             7511
_exptl_crystal_size_max          0.066
_exptl_crystal_size_mid          0.056
_exptl_crystal_size_min          0.038
_refine_diff_density_max         1.416
_refine_diff_density_min         -1.174
_refine_diff_density_rms         0.304
_refine_ls_extinction_coef       .
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.018
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     80
_refine_ls_number_reflns         2164
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.018
_refine_ls_R_factor_all          0.1447
_refine_ls_R_factor_gt           0.0655
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+174.9007P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1145
_refine_ls_wR_factor_ref         0.1437
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_full    .
_reflns_Friedel_fraction_max     .
_reflns_number_gt                1106
_reflns_number_total             2164
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            JSSC-2019-120990.cif
_cod_data_source_block           III
_cod_original_cell_volume        6100(3)
_cod_original_sg_symbol_H-M      'I 41/a c d'
_cod_database_code               1561653
_shelx_shelxl_version_number     2018/3
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_shelx_estimated_absorpt_t_max   0.332
_shelx_estimated_absorpt_t_min   0.193
_olex2_refinement_description
;
1. Uiso/Uaniso restraints and constraints
Uanis(Sr4A) = Uanis(Sr4B)
Uanis(Sr2A) = Uanis(Sr2B)
2. Others
 Sof(Sr2B)=Sof(Sr4B)=1-FVAR(1)
 Sof(Sr2A)=Sof(Sr4A)=FVAR(1)
 Fixed Sof: As4(0.25)
;
_olex2_submission_special_instructions 'No special instructions were received'
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x+1/2, -y, z+1/2'
'-y+1/4, x+3/4, z+1/4'
'y+1/4, -x+1/4, z+3/4'
'-x+1/2, y, -z'
'x, -y, -z+1/2'
'y+1/4, x+3/4, -z+3/4'
'-y+1/4, -x+1/4, -z+1/4'
'x+1/2, y+1/2, z+1/2'
'-x+1, -y+1/2, z+1'
'-y+3/4, x+5/4, z+3/4'
'y+3/4, -x+3/4, z+5/4'
'-x+1, y+1/2, -z+1/2'
'x+1/2, -y+1/2, -z+1'
'y+3/4, x+5/4, -z+5/4'
'-y+3/4, -x+3/4, -z+3/4'
'-x, -y, -z'
'x-1/2, y, -z-1/2'
'y-1/4, -x-3/4, -z-1/4'
'-y-1/4, x-1/4, -z-3/4'
'x-1/2, -y, z'
'-x, y, z-1/2'
'-y-1/4, -x-3/4, z-3/4'
'y-1/4, x-1/4, z-1/4'
'-x+1/2, -y+1/2, -z+1/2'
'x, y+1/2, -z'
'y+1/4, -x-1/4, -z+1/4'
'-y+1/4, x+1/4, -z-1/4'
'x, -y+1/2, z+1/2'
'-x+1/2, y+1/2, z'
'-y+1/4, -x-1/4, z-1/4'
'y+1/4, x+1/4, z+1/4'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Sr1 Sr 0.04496(9) 0.07152(9) 0.17125(6) 0.0389(4) Uani 1 1 d . . . . .
Sr2A Sr 0.02335(12) 0.37570(13) 0.00327(10) 0.0365(5) Uani 0.860(4) 1 d . . . .
.
Sr2B Sr 0.0088(9) 0.3633(9) 0.0232(7) 0.0365(5) Uani 0.140(4) 1 d . . . . .
Sr3 Sr 0.35471(13) 0.000000 0.250000 0.0418(5) Uani 1 2 d S T P . .
Sr4A Sr 0.34965(12) 0.07137(11) 0.09515(8) 0.0393(5) Uani 0.860(4) 1 d . . . .
.
Sr4B Sr 0.3189(8) 0.0413(7) 0.0712(5) 0.0393(5) Uani 0.140(4) 1 d . . . . .
Zn1 Zn 0.000000 0.250000 0.375000 0.0515(10) Uani 1 4 d S T P . .
Zn2 Zn 0.3659(11) 0.1763(13) 0.1497(8) 0.058(8) Uani 0.115(8) 1 d . . . . .
As1 As 0.13247(9) 0.38247(9) 0.125000 0.0353(5) Uani 1 2 d S T P . .
As2 As 0.36567(9) 0.25170(9) 0.05821(7) 0.0358(4) Uani 1 1 d . . . . .
As3 As 0.12967(11) 0.02269(10) 0.04718(7) 0.0432(4) Uani 1 1 d . . . . .
As4 As 0.01575(16) 0.26575(16) 0.125000 0.0373(12) Uani 0.5 2 d S T P . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
As As 0.0499 2.0058 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Sr Sr -1.5307 3.2498 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Zn Zn 0.2839 1.4301 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
Sr2B Sr1 Sr2B 98.1(4) 15_444 10_454
Sr2B Sr1 Sr4A 121.9(3) 15_444 8
Sr2B Sr1 Sr4A 107.0(3) 10_454 8
Sr2B Sr1 Sr4B 108.2(3) 15_444 8
Sr4B Sr1 Sr2B 115.2(3) 8 10_454
Sr4B Sr1 Sr4A 14.2(2) 8 8
Zn2 Sr1 Sr2B 83.2(4) 8 10_454
Zn2 Sr1 Sr2B 153.0(4) 8 15_444
Zn2 Sr1 Sr4A 34.9(3) 8 8
Zn2 Sr1 Sr4B 49.1(4) 8 8
As1 Sr1 Sr2B 101.5(3) 10_454 15_444
As1 Sr1 Sr2B 53.5(3) 10_454 10_454
As1 Sr1 Sr4A 135.58(6) 10_454 8
As1 Sr1 Sr4B 149.8(2) 10_454 8
As1 Sr1 Zn2 100.8(3) 10_454 8
As1 Sr1 As2 91.97(5) 10_454 3_545
As1 Sr1 As2 93.15(6) 10_454 8
As1 Sr1 As3 100.33(5) 10_454 .
As1 Sr1 As4 63.14(7) 10_454 .
As2 Sr1 Sr2B 62.9(3) 3_545 15_444
As2 Sr1 Sr2B 150.5(3) 8 15_444
As2 Sr1 Sr2B 138.1(3) 3_545 10_454
As2 Sr1 Sr2B 111.1(2) 8 10_454
As2 Sr1 Sr4A 53.71(5) 8 8
As2 Sr1 Sr4A 114.71(6) 3_545 8
As2 Sr1 Sr4B 106.4(2) 3_545 8
As2 Sr1 Sr4B 63.3(2) 8 8
As2 Sr1 Zn2 41.4(3) 8 8
As2 Sr1 Zn2 131.1(3) 3_545 8
As2 Sr1 As2 91.39(5) 8 3_545
As2 Sr1 As4 92.38(5) 3_545 .
As2 Sr1 As4 156.10(8) 8 .
As3 Sr1 Sr2B 52.2(3) . 10_454
As3 Sr1 Sr2B 53.0(3) 8 15_444
As3 Sr1 Sr2B 112.7(3) . 15_444
As3 Sr1 Sr2B 111.1(3) 8 10_454
As3 Sr1 Sr4A 69.10(5) 8 8
As3 Sr1 Sr4A 56.52(5) . 8
As3 Sr1 Sr4B 55.9(2) 8 8
As3 Sr1 Sr4B 63.06(19) . 8
As3 Sr1 Zn2 101.2(4) 8 8
As3 Sr1 Zn2 47.9(3) . 8
As3 Sr1 As1 150.99(7) 8 10_454
As3 Sr1 As2 115.86(6) 8 8
As3 Sr1 As2 167.63(7) . 3_545
As3 Sr1 As2 89.22(5) . 8
As3 Sr1 As2 87.62(5) 8 3_545
As3 Sr1 As3 81.01(6) 8 .
As3 Sr1 As4 87.88(7) 8 .
As3 Sr1 As4 92.05(5) . .
As4 Sr1 Sr2B 48.9(2) 10_454 10_454
As4 Sr1 Sr2B 56.7(3) 10_454 15_444
As4 Sr1 Sr2B 47.5(3) . 15_444
As4 Sr1 Sr2B 53.3(2) . 10_454
As4 Sr1 Sr4A 149.08(6) 10_454 8
As4 Sr1 Sr4A 142.61(6) . 8
As4 Sr1 Sr4B 147.0(2) 10_454 8
As4 Sr1 Sr4B 137.3(2) . 8
As4 Sr1 Zn2 131.9(3) 10_454 8
As4 Sr1 Zn2 135.4(3) . 8
As4 Sr1 As1 51.67(8) 10_454 10_454
As4 Sr1 As2 92.53(5) 10_454 3_545
As4 Sr1 As2 144.70(9) 10_454 8
As4 Sr1 As3 99.35(8) 10_454 8
As4 Sr1 As3 94.10(5) 10_454 .
As4 Sr1 As4 11.47(12) 10_454 .
Sr2B Sr2A Sr3 119.1(19) . 27_565
Sr2B Sr2A Sr4A 103.4(18) . 14_454
Sr2B Sr2A Zn1 113.0(18) . 29_554
Sr2B Sr2A Zn2 159.4(19) . 31_565
Sr2B Sr2A As1 64.9(18) . .
Sr2B Sr2A As2 77.0(18) . 14_454
Sr2B Sr2A As2 112.2(18) . 5
Sr2B Sr2A As3 66.3(18) . 10_454
Sr2B Sr2A As3 144.4(18) . 26
Sr2B Sr2A As4 25.4(18) . .
Sr2B Sr2A As4 21.9(18) . 10_454
Sr4A Sr2A Sr3 137.42(7) 14_454 27_565
Zn1 Sr2A Sr3 98.18(5) 29_554 27_565
Zn1 Sr2A Sr4A 64.97(5) 29_554 14_454
Zn1 Sr2A As2 43.72(3) 29_554 14_454
Zn1 Sr2A As4 102.06(7) 29_554 10_454
Zn2 Sr2A Sr3 68.9(5) 31_565 27_565
Zn2 Sr2A Sr4A 72.0(5) 31_565 14_454
Zn2 Sr2A Zn1 46.6(4) 31_565 29_554
Zn2 Sr2A As1 126.5(5) 31_565 .
Zn2 Sr2A As2 85.3(4) 31_565 14_454
Zn2 Sr2A As2 54.2(4) 31_565 5
Zn2 Sr2A As3 121.8(5) 31_565 10_454
Zn2 Sr2A As3 56.0(4) 31_565 26
Zn2 Sr2A As4 142.9(4) 31_565 10_454
Zn2 Sr2A As4 145.6(4) 31_565 .
As1 Sr2A Sr3 57.58(4) . 27_565
As1 Sr2A Sr4A 155.57(7) . 14_454
As1 Sr2A Zn1 138.67(7) . 29_554
As1 Sr2A As2 137.18(8) . 14_454
As1 Sr2A As4 59.81(7) . 10_454
As1 Sr2A As4 49.25(8) . .
As2 Sr2A Sr3 56.94(5) 5 27_565
As2 Sr2A Sr3 139.40(7) 14_454 27_565
As2 Sr2A Sr4A 49.98(5) 14_454 14_454
As2 Sr2A Sr4A 110.59(7) 5 14_454
As2 Sr2A Zn1 46.83(4) 5 29_554
As2 Sr2A As1 93.83(6) 5 .
As2 Sr2A As2 82.63(6) 5 14_454
As2 Sr2A As3 91.17(7) 5 26
As2 Sr2A As3 163.99(8) 5 10_454
As2 Sr2A As4 91.46(6) 5 .
As2 Sr2A As4 77.52(7) 14_454 10_454
As2 Sr2A As4 90.74(6) 5 10_454
As3 Sr2A Sr3 51.80(5) 26 27_565
As3 Sr2A Sr3 138.61(8) 10_454 27_565
As3 Sr2A Sr4A 92.07(7) 26 14_454
As3 Sr2A Sr4A 56.46(6) 10_454 14_454
As3 Sr2A Zn1 102.55(7) 26 29_554
As3 Sr2A Zn1 117.97(7) 10_454 29_554
As3 Sr2A As1 99.35(7) 10_454 .
As3 Sr2A As1 88.01(7) 26 .
As3 Sr2A As2 134.54(8) 26 14_454
As3 Sr2A As2 81.53(6) 10_454 14_454
As3 Sr2A As3 98.29(7) 10_454 26
As3 Sr2A As4 137.26(10) 26 .
As3 Sr2A As4 88.10(6) 10_454 10_454
As3 Sr2A As4 147.82(9) 26 10_454
As3 Sr2A As4 90.31(6) 10_454 .
As4 Sr2A Sr3 104.25(7) 10_454 27_565
As4 Sr2A Sr3 95.86(7) . 27_565
As4 Sr2A Sr4A 126.35(8) . 14_454
As4 Sr2A Sr4A 117.13(7) 10_454 14_454
As4 Sr2A Zn1 110.02(8) . 29_554
As4 Sr2A As2 88.05(8) . 14_454
As4 Sr2A As4 10.56(11) . 10_454
Sr1 Sr2B Sr1 63.5(2) 15_444 10_454
Sr1 Sr2B Sr2B 106.2(3) 10_454 10_454
Sr1 Sr2B Sr2B 67.2(4) 15_444 10_454
Sr1 Sr2B As2 54.7(2) 15_444 14_454
Sr1 Sr2B As3 149.5(5) 15_444 26
Sr1 Sr2B As3 108.4(4) 10_454 26
Sr2A Sr2B Sr1 138(2) . 10_454
Sr2A Sr2B Sr1 143(2) . 15_444
Sr2A Sr2B Sr2B 114.1(18) . 10_454
Sr2A Sr2B Zn2 16.9(15) . 31_565
Sr2A Sr2B As1 105.9(19) . .
Sr2A Sr2B As2 59.0(17) . 5
Sr2A Sr2B As2 94.3(19) . 14_454
Sr2A Sr2B As3 104.2(19) . 10_454
Sr2A Sr2B As3 30.6(16) . 26
Sr2A Sr2B As4 150(2) . .
Sr2A Sr2B As4 154(2) . 10_454
Zn2 Sr2B Sr1 132.8(6) 31_565 15_444
Zn2 Sr2B Sr1 155.2(6) 31_565 10_454
Zn2 Sr2B Sr2B 98.2(5) 31_565 10_454
Zn2 Sr2B As1 115.8(6) 31_565 .
Zn2 Sr2B As2 48.0(4) 31_565 5
Zn2 Sr2B As2 79.9(5) 31_565 14_454
Zn2 Sr2B As3 111.5(6) 31_565 10_454
Zn2 Sr2B As3 47.4(4) 31_565 26
Zn2 Sr2B As4 142.6(6) 31_565 10_454
As1 Sr2B Sr1 56.7(3) . 10_454
As1 Sr2B Sr1 110.8(4) . 15_444
As1 Sr2B Sr2B 98.9(5) . 10_454
As1 Sr2B As2 151.7(5) . 14_454
As1 Sr2B As2 92.8(4) . 5
As1 Sr2B As3 83.2(4) . 26
As1 Sr2B As4 67.6(3) . 10_454
As2 Sr2B Sr1 145.7(5) 5 10_454
As2 Sr2B Sr1 124.4(5) 5 15_444
As2 Sr2B Sr1 118.1(4) 14_454 10_454
As2 Sr2B Sr2B 54.1(3) 14_454 10_454
As2 Sr2B Sr2B 59.6(4) 5 10_454
As2 Sr2B As2 80.6(3) 5 14_454
As2 Sr2B As3 121.9(4) 14_454 26
As2 Sr2B As3 79.8(3) 5 26
As3 Sr2B Sr1 58.0(3) 10_454 15_444
As3 Sr2B Sr1 57.4(3) 10_454 10_454
As3 Sr2B Sr2B 124.4(7) 10_454 10_454
As3 Sr2B Sr2B 139.4(5) 26 10_454
As3 Sr2B As1 108.0(5) 10_454 .
As3 Sr2B As2 85.4(4) 10_454 14_454
As3 Sr2B As2 156.9(5) 10_454 5
As3 Sr2B As3 92.4(4) 10_454 26
As3 Sr2B As4 101.4(4) 10_454 10_454
As4 Sr2B Sr1 55.4(3) . 10_454
As4 Sr2B Sr1 54.1(2) 10_454 15_444
As4 Sr2B Sr1 60.3(2) 10_454 10_454
As4 Sr2B Sr1 64.1(3) . 15_444
As4 Sr2B Sr2B 55.1(3) . 10_454
As4 Sr2B Sr2B 46.7(3) 10_454 10_454
As4 Sr2B Zn2 143.8(7) . 31_565
As4 Sr2B As1 55.1(3) . .
As4 Sr2B As2 85.6(4) 10_454 14_454
As4 Sr2B As2 95.8(4) . 5
As4 Sr2B As2 95.8(4) 10_454 5
As4 Sr2B As2 97.9(4) . 14_454
As4 Sr2B As3 138.0(6) . 26
As4 Sr2B As3 150.4(5) 10_454 26
As4 Sr2B As3 104.3(4) . 10_454
As4 Sr2B As4 12.50(14) . 10_454
Sr4A Sr3 Sr4A 177.38(9) 6 .
Sr4A Sr3 Zn2 146.4(3) . 6
Sr4A Sr3 Zn2 146.4(3) 6 .
Sr4A Sr3 Zn2 33.8(3) . .
Sr4A Sr3 Zn2 33.8(3) 6 6
Sr4B Sr3 Sr4A 110.5(2) 8 6
Sr4B Sr3 Sr4A 67.34(19) 3_545 6
Sr4B Sr3 Sr4A 110.5(2) 3_545 .
Sr4B Sr3 Sr4A 67.34(19) 8 .
Sr4B Sr3 Sr4B 78.2(4) 8 3_545
Sr4B Sr3 Zn2 93.6(3) 8 6
Sr4B Sr3 Zn2 90.9(4) 3_545 6
Sr4B Sr3 Zn2 90.9(4) 8 .
Sr4B Sr3 Zn2 93.6(3) 3_545 .
Sr4B Sr3 As1 54.5(2) 3_545 25
Sr4B Sr3 As1 132.6(2) 8 25
Sr4B Sr3 As1 132.6(2) 3_545 20_656
Sr4B Sr3 As1 54.5(2) 8 20_656
Sr4B Sr3 As2 123.1(2) 3_545 20_656
Sr4B Sr3 As2 123.1(2) 8 23_666
Sr4B Sr3 As2 124.4(2) 3_545 23_666
Sr4B Sr3 As2 124.4(2) 8 20_656
Zn2 Sr3 Zn2 174.2(6) . 6
As1 Sr3 Sr4A 126.44(4) 20_656 6
As1 Sr3 Sr4A 53.76(4) 25 6
As1 Sr3 Sr4A 53.76(4) 20_656 .
As1 Sr3 Sr4A 126.45(4) 25 .
As1 Sr3 Zn2 92.7(3) 25 .
As1 Sr3 Zn2 87.0(3) 25 6
As1 Sr3 Zn2 92.7(3) 20_656 6
As1 Sr3 Zn2 87.0(3) 20_656 .
As1 Sr3 As1 172.88(9) 25 20_656
As2 Sr3 Sr4A 57.21(4) 20_656 .
As2 Sr3 Sr4A 125.05(6) 20_656 6
As2 Sr3 Sr4A 57.21(4) 23_666 6
As2 Sr3 Sr4A 125.05(6) 23_666 .
As2 Sr3 Zn2 131.3(3) 20_656 6
As2 Sr3 Zn2 131.3(3) 23_666 .
As2 Sr3 Zn2 42.9(3) 23_666 6
As2 Sr3 Zn2 42.9(3) 20_656 .
As2 Sr3 As1 87.11(5) 20_656 25
As2 Sr3 As1 87.79(4) 20_656 20_656
As2 Sr3 As1 87.11(5) 23_666 20_656
As2 Sr3 As1 87.79(4) 23_666 25
As2 Sr3 As2 88.54(7) 20_656 23_666
As3 Sr3 Sr4A 121.09(6) 3_545 .
As3 Sr3 Sr4A 56.80(4) 3_545 6
As3 Sr3 Sr4A 56.80(4) 8 .
As3 Sr3 Sr4A 121.09(6) 8 6
As3 Sr3 Sr4B 53.8(2) 8 3_545
As3 Sr3 Sr4B 62.0(2) 8 8
As3 Sr3 Sr4B 62.0(2) 3_545 3_545
As3 Sr3 Sr4B 53.8(2) 3_545 8
As3 Sr3 Zn2 46.8(3) 3_545 6
As3 Sr3 Zn2 138.9(3) 3_545 .
As3 Sr3 Zn2 138.9(3) 8 6
As3 Sr3 Zn2 46.8(3) 8 .
As3 Sr3 As1 97.39(5) 3_545 25
As3 Sr3 As1 97.39(5) 8 20_656
As3 Sr3 As1 87.48(4) 8 25
As3 Sr3 As1 87.48(4) 3_545 20_656
As3 Sr3 As2 88.98(4) 8 20_656
As3 Sr3 As2 174.77(5) 8 23_666
As3 Sr3 As2 88.98(4) 3_545 23_666
As3 Sr3 As2 174.77(5) 3_545 20_656
As3 Sr3 As3 93.84(9) 3_545 8
Sr1 Sr4A Sr2A 113.61(6) 8 14_554
Sr1 Sr4A Sr3 108.14(5) 8 .
Sr1 Sr4A Sr4B 86.72(18) 8 8
Sr1 Sr4A Zn2 130.7(3) 8 20_656
Sr2A Sr4A Sr4B 155.8(2) 14_554 8
Sr2A Sr4A Zn2 38.4(3) 14_554 20_656
Sr3 Sr4A Sr2A 128.18(7) . 14_554
Sr3 Sr4A Sr4B 49.3(2) . 8
Sr3 Sr4A Zn2 90.7(3) . 20_656
Sr4B Sr4A Sr1 80.4(7) . 8
Sr4B Sr4A Sr2A 102.5(7) . 14_554
Sr4B Sr4A Sr3 113.7(7) . .
Sr4B Sr4A Sr4B 66.6(8) . 8
Sr4B Sr4A Zn2 150.3(9) . .
Sr4B Sr4A Zn2 133.4(8) . 20_656
Sr4B Sr4A As1 68.5(7) . 20_656
Sr4B Sr4A As2 115.2(7) . .
Sr4B Sr4A As2 158.1(7) . 20_656
Sr4B Sr4A As3 48.9(7) . 5
Sr4B Sr4A As3 103.3(7) . 8
Zn2 Sr4A Sr1 70.1(5) . 8
Zn2 Sr4A Sr2A 92.9(4) . 14_554
Zn2 Sr4A Sr3 73.6(5) . .
Zn2 Sr4A Sr4B 135.1(4) 20_656 8
Zn2 Sr4A Sr4B 107.0(5) . 8
Zn2 Sr4A Zn2 72.6(7) . 20_656
Zn2 Sr4A As1 131.2(5) . 20_656
Zn2 Sr4A As2 50.4(5) . 20_656
Zn2 Sr4A As2 50.4(5) . .
Zn2 Sr4A As3 56.8(4) . 8
Zn2 Sr4A As3 137.3(5) . 5
As1 Sr4A Sr1 133.60(7) 20_656 8
As1 Sr4A Sr2A 106.32(6) 20_656 14_554
As1 Sr4A Sr3 59.14(3) 20_656 .
As1 Sr4A Sr4B 49.96(18) 20_656 8
As1 Sr4A Zn2 95.3(3) 20_656 20_656
As1 Sr4A As2 90.61(6) 20_656 20_656
As1 Sr4A As3 98.35(6) 20_656 8
As1 Sr4A As3 87.38(6) 20_656 5
As2 Sr4A Sr1 56.77(5) . 8
As2 Sr4A Sr1 120.41(7) 20_656 8
As2 Sr4A Sr2A 63.32(6) . 14_554
As2 Sr4A Sr2A 76.44(6) 20_656 14_554
As2 Sr4A Sr3 56.16(5) 20_656 .
As2 Sr4A Sr3 124.01(7) . .
As2 Sr4A Sr4B 140.62(19) . 8
As2 Sr4A Sr4B 105.4(2) 20_656 8
As2 Sr4A Zn2 74.8(3) . 20_656
As2 Sr4A Zn2 38.7(3) 20_656 20_656
As2 Sr4A As1 169.26(8) . 20_656
As2 Sr4A As2 84.25(7) . 20_656
As2 Sr4A As3 88.17(6) . 5
As2 Sr4A As3 90.66(6) . 8
As3 Sr4A Sr1 55.59(5) 8 8
As3 Sr4A Sr1 97.59(6) 5 8
As3 Sr4A Sr2A 53.61(5) 5 14_554
As3 Sr4A Sr2A 149.37(8) 8 14_554
As3 Sr4A Sr3 52.57(5) 8 .
As3 Sr4A Sr3 146.29(6) 5 .
As3 Sr4A Sr4B 53.3(2) 8 8
As3 Sr4A Sr4B 113.1(3) 5 8
As3 Sr4A Zn2 88.6(3) 5 20_656
As3 Sr4A Zn2 122.6(2) 8 20_656
As3 Sr4A As2 85.59(6) 8 20_656
As3 Sr4A As2 126.82(7) 5 20_656
As3 Sr4A As3 147.20(9) 8 5
Sr1 Sr4B Sr4A 92.6(3) 8 8
Sr1 Sr4B Sr4B 70.1(3) 8 5
Sr1 Sr4B As2 53.61(16) 8 .
Sr3 Sr4B Sr1 112.0(4) 4_554 8
Sr3 Sr4B Sr4A 63.3(2) 4_554 8
Sr3 Sr4B Sr4B 76.1(5) 4_554 8
Sr3 Sr4B Sr4B 50.9(2) 4_554 5
Sr3 Sr4B As2 142.4(4) 4_554 .
Sr3 Sr4B As3 123.6(4) 4_554 8
Sr3 Sr4B As3 58.6(3) 4_554 .
Sr4A Sr4B Sr1 85.4(7) . 8
Sr4A Sr4B Sr3 162.1(9) . 4_554
Sr4A Sr4B Sr4A 113.4(8) . 8
Sr4A Sr4B Sr4B 145.2(7) . 5
Sr4A Sr4B Sr4B 100.0(9) . 8
Sr4A Sr4B Sr4B 92.7(4) 8 5
Sr4A Sr4B Zn2 21.1(6) . .
Sr4A Sr4B As1 95.4(8) . 20_656
Sr4A Sr4B As2 51.8(6) . .
Sr4A Sr4B As3 135.7(9) . .
Sr4A Sr4B As3 62.6(7) . 8
Sr4A Sr4B As3 117.2(9) . 5
Sr4B Sr4B Sr1 91.36(17) 8 8
Sr4B Sr4B Sr4A 13.4(3) 8 8
Sr4B Sr4B Sr4B 104.8(5) 8 5
Sr4B Sr4B As2 132.1(4) 8 .
Sr4B Sr4B As3 53.5(3) 8 8
Zn2 Sr4B Sr1 64.5(4) . 8
Zn2 Sr4B Sr3 172.3(5) . 4_554
Zn2 Sr4B Sr4A 109.5(4) . 8
Zn2 Sr4B Sr4B 129.7(4) . 5
Zn2 Sr4B Sr4B 96.9(6) . 8
Zn2 Sr4B As1 110.7(6) . 20_656
Zn2 Sr4B As2 41.8(4) . .
Zn2 Sr4B As3 48.7(4) . 8
Zn2 Sr4B As3 115.6(5) . .
As1 Sr4B Sr1 145.0(4) 20_656 8
As1 Sr4B Sr3 67.9(3) 20_656 4_554
As1 Sr4B Sr4A 54.99(18) 20_656 8
As1 Sr4B Sr4B 118.8(3) 20_656 5
As1 Sr4B Sr4B 54.0(2) 20_656 8
As1 Sr4B As2 145.8(5) 20_656 .
As1 Sr4B As3 95.9(3) 20_656 8
As1 Sr4B As3 104.3(4) 20_656 .
As2 Sr4B Sr4A 140.5(3) . 8
As2 Sr4B Sr4B 93.4(2) . 5
As3 Sr4B Sr1 109.0(3) 5 8
As3 Sr4B Sr1 53.58(16) 8 8
As3 Sr4B Sr1 56.17(19) . 8
As3 Sr4B Sr3 62.6(3) 5 4_554
As3 Sr4B Sr4A 54.8(2) . 8
As3 Sr4B Sr4A 125.9(5) 5 8
As3 Sr4B Sr4A 63.64(18) 8 8
As3 Sr4B Sr4B 115.2(4) 8 5
As3 Sr4B Sr4B 138.3(7) 5 8
As3 Sr4B Sr4B 53.6(3) 5 5
As3 Sr4B Sr4B 63.8(3) . 8
As3 Sr4B Sr4B 45.0(3) . 5
As3 Sr4B Zn2 124.6(5) 5 .
As3 Sr4B As1 101.7(3) 5 20_656
As3 Sr4B As2 107.0(3) . .
As3 Sr4B As2 78.6(3) 8 .
As3 Sr4B As2 87.9(3) 5 .
As3 Sr4B As3 76.0(2) . 8
As3 Sr4B As3 162.2(4) 5 8
As3 Sr4B As3 97.3(4) 5 .
Sr2A Zn1 Sr2A 130.44(5) 15_444 29
Sr2A Zn1 Sr2A 72.70(7) 22_556 29
Sr2A Zn1 Sr2A 72.70(7) 8 15_444
Sr2A Zn1 Sr2A 130.44(5) 22_556 15_444
Sr2A Zn1 Sr2A 130.44(5) 8 22_556
Sr2A Zn1 Sr2A 130.44(5) 8 29
Zn2 Zn1 Sr2A 89.4(4) 12_454 8
Zn2 Zn1 Sr2A 89.4(4) 18_556 29
Zn2 Zn1 Sr2A 110.7(4) 18_556 22_556
Zn2 Zn1 Sr2A 110.7(4) 3_545 8
Zn2 Zn1 Sr2A 112.2(4) 25 8
Zn2 Zn1 Sr2A 112.2(4) 18_556 15_444
Zn2 Zn1 Sr2A 112.2(4) 12_454 29
Zn2 Zn1 Sr2A 43.8(4) 25 15_444
Zn2 Zn1 Sr2A 110.7(4) 25 29
Zn2 Zn1 Sr2A 110.7(4) 12_454 15_444
Zn2 Zn1 Sr2A 89.4(4) 3_545 15_444
Zn2 Zn1 Sr2A 89.4(4) 25 22_556
Zn2 Zn1 Sr2A 43.8(4) 18_556 8
Zn2 Zn1 Sr2A 43.8(4) 12_454 22_556
Zn2 Zn1 Sr2A 112.2(4) 3_545 22_556
Zn2 Zn1 Sr2A 43.8(4) 3_545 29
Zn2 Zn1 Zn2 155.3(8) 18_556 25
Zn2 Zn1 Zn2 92.61(17) 25 3_545
Zn2 Zn1 Zn2 92.61(17) 18_556 3_545
Zn2 Zn1 Zn2 92.61(17) 18_556 12_454
Zn2 Zn1 Zn2 92.61(17) 25 12_454
Zn2 Zn1 Zn2 155.3(8) 12_454 3_545
Zn2 Zn1 As2 58.8(4) 12_454 18_556
Zn2 Zn1 As2 58.8(4) 3_545 25
Zn2 Zn1 As2 145.5(4) 18_556 25
Zn2 Zn1 As2 106.3(4) 18_556 12_454
Zn2 Zn1 As2 54.1(4) 3_545 3_545
Zn2 Zn1 As2 58.8(4) 25 12_454
Zn2 Zn1 As2 54.1(4) 25 25
Zn2 Zn1 As2 145.5(4) 3_545 12_454
Zn2 Zn1 As2 106.3(4) 3_545 18_556
Zn2 Zn1 As2 54.1(4) 18_556 18_556
Zn2 Zn1 As2 54.1(4) 12_454 12_454
Zn2 Zn1 As2 58.8(4) 18_556 3_545
Zn2 Zn1 As2 145.5(4) 25 18_556
Zn2 Zn1 As2 106.3(4) 25 3_545
Zn2 Zn1 As2 145.5(4) 12_454 3_545
Zn2 Zn1 As2 106.3(4) 12_454 25
As2 Zn1 Sr2A 69.27(5) 12_454 8
As2 Zn1 Sr2A 88.14(5) 3_545 29
As2 Zn1 Sr2A 69.27(5) 25 22_556
As2 Zn1 Sr2A 88.14(5) 18_556 8
As2 Zn1 Sr2A 158.76(5) 12_454 29
As2 Zn1 Sr2A 69.27(5) 3_545 15_444
As2 Zn1 Sr2A 56.93(5) 18_556 22_556
As2 Zn1 Sr2A 88.14(5) 25 15_444
As2 Zn1 Sr2A 158.76(5) 25 8
As2 Zn1 Sr2A 56.93(5) 12_454 15_444
As2 Zn1 Sr2A 69.27(5) 18_556 29
As2 Zn1 Sr2A 158.76(5) 18_556 15_444
As2 Zn1 Sr2A 88.14(5) 12_454 22_556
As2 Zn1 Sr2A 56.93(5) 3_545 8
As2 Zn1 Sr2A 158.76(5) 3_545 22_556
As2 Zn1 Sr2A 56.93(5) 25 29
As2 Zn1 As2 112.09(7) 25 18_556
As2 Zn1 As2 108.18(3) 3_545 25
As2 Zn1 As2 108.18(3) 12_454 18_556
As2 Zn1 As2 112.09(7) 3_545 12_454
As2 Zn1 As2 108.18(3) 25 12_454
As2 Zn1 As2 108.18(3) 3_545 18_556
Sr1 Zn2 Sr3 109.8(5) 8 .
Sr1 Zn2 Sr4A 73.1(4) 8 27_565
Sr2A Zn2 Sr1 115.4(6) 23_666 8
Sr2A Zn2 Sr2B 3.7(3) 23_666 23_666
Sr2A Zn2 Sr3 72.4(4) 23_666 .
Sr2A Zn2 Sr4A 69.6(5) 23_666 27_565
Sr2A Zn2 Sr4B 146.2(8) 23_666 .
Sr2A Zn2 Zn1 89.6(7) 23_666 25
Sr2A Zn2 As2 75.0(5) 23_666 20_656
Sr2A Zn2 As3 75.7(4) 23_666 8
Sr2B Zn2 Sr1 118.1(6) 23_666 8
Sr2B Zn2 Sr3 74.1(5) 23_666 .
Sr2B Zn2 Sr4A 69.0(5) 23_666 27_565
Sr3 Zn2 Sr4A 138.3(5) . 27_565
Sr4A Zn2 Sr1 75.0(5) . 8
Sr4A Zn2 Sr2A 144.8(9) . 23_666
Sr4A Zn2 Sr2B 146.6(9) . 23_666
Sr4A Zn2 Sr3 72.6(5) . .
Sr4A Zn2 Sr4A 142.0(7) . 27_565
Sr4A Zn2 Sr4B 8.6(3) . .
Sr4A Zn2 Zn1 111.6(7) . 25
Sr4A Zn2 As2 86.2(6) . .
Sr4A Zn2 As2 90.0(7) . 20_656
Sr4A Zn2 As3 82.5(6) . 8
Sr4B Zn2 Sr1 66.4(5) . 8
Sr4B Zn2 Sr2B 148.8(8) . 23_666
Sr4B Zn2 Sr3 75.6(5) . .
Sr4B Zn2 Sr4A 135.2(6) . 27_565
Zn1 Zn2 Sr1 126.5(6) 25 8
Zn1 Zn2 Sr2B 86.0(7) 25 23_666
Zn1 Zn2 Sr3 123.1(6) 25 .
Zn1 Zn2 Sr4A 73.3(5) 25 27_565
Zn1 Zn2 Sr4B 117.1(6) 25 .
Zn1 Zn2 As3 165.2(8) 25 8
As2 Zn2 Sr1 62.7(4) . 8
As2 Zn2 Sr1 164.5(8) 20_656 8
As2 Zn2 Sr2A 128.8(9) . 23_666
As2 Zn2 Sr2B 127.2(9) . 23_666
As2 Zn2 Sr2B 72.8(6) 20_656 23_666
As2 Zn2 Sr3 158.8(8) . .
As2 Zn2 Sr3 60.9(4) 20_656 .
As2 Zn2 Sr4A 61.0(4) . 27_565
As2 Zn2 Sr4A 122.3(7) 20_656 27_565
As2 Zn2 Sr4B 83.3(6) . .
As2 Zn2 Sr4B 98.5(7) 20_656 .
As2 Zn2 Zn1 62.3(4) 20_656 25
As2 Zn2 Zn1 64.8(4) . 25
As2 Zn2 As2 121.0(6) . 20_656
As2 Zn2 As3 114.7(6) 20_656 8
As2 Zn2 As3 123.0(7) . 8
As3 Zn2 Sr1 60.3(4) 8 8
As3 Zn2 Sr2B 79.4(5) 8 23_666
As3 Zn2 Sr3 55.0(3) 8 .
As3 Zn2 Sr4A 98.9(5) 8 27_565
As3 Zn2 Sr4B 77.4(6) 8 .
Sr1 As1 Sr1 122.66(9) 8 10_454
Sr1 As1 Sr2A 76.84(5) 10_454 .
Sr1 As1 Sr2A 80.22(5) 10_454 15_444
Sr1 As1 Sr2A 76.84(5) 8 15_444
Sr1 As1 Sr2A 80.22(5) 8 .
Sr1 As1 Sr3 69.91(4) 10_454 25
Sr1 As1 Sr3 140.51(3) 8 25
Sr1 As1 Sr4A 143.38(6) 10_454 27_565
Sr1 As1 Sr4A 143.38(6) 8 30
Sr1 As1 Sr4A 85.44(5) 8 27_565
Sr1 As1 Sr4A 85.44(5) 10_454 30
Sr2A As1 Sr2A 131.06(10) 15_444 .
Sr2A As1 Sr3 137.47(5) . 25
Sr2A As1 Sr3 68.46(4) 15_444 25
Sr2B As1 Sr1 69.8(3) . 10_454
Sr2B As1 Sr1 79.9(3) . 8
Sr2B As1 Sr1 69.8(3) 15_444 8
Sr2B As1 Sr1 79.9(3) 15_444 10_454
Sr2B As1 Sr2A 122.5(3) 15_444 .
Sr2B As1 Sr2A 9.3(2) . .
Sr2B As1 Sr2A 9.3(2) 15_444 15_444
Sr2B As1 Sr2A 122.5(3) . 15_444
Sr2B As1 Sr2B 114.3(5) . 15_444
Sr2B As1 Sr3 77.1(3) 15_444 25
Sr2B As1 Sr3 135.0(3) . 25
Sr2B As1 Sr4A 90.4(3) . 30
Sr2B As1 Sr4A 90.4(3) 15_444 27_565
Sr2B As1 Sr4A 144.2(3) . 27_565
Sr2B As1 Sr4A 144.2(3) 15_444 30
Sr4A As1 Sr2A 84.86(5) 30 .
Sr4A As1 Sr2A 135.56(6) 27_565 .
Sr4A As1 Sr2A 84.86(5) 27_565 15_444
Sr4A As1 Sr2A 135.56(6) 30 15_444
Sr4A As1 Sr3 73.52(6) 27_565 25
Sr4A As1 Sr3 67.10(5) 30 25
Sr4A As1 Sr4A 82.18(8) 27_565 30
Sr4B As1 Sr1 127.5(3) 30 8
Sr4B As1 Sr1 99.6(3) 27_565 8
Sr4B As1 Sr1 99.6(3) 30 10_454
Sr4B As1 Sr1 127.5(3) 27_565 10_454
Sr4B As1 Sr2A 145.8(2) 27_565 .
Sr4B As1 Sr2A 81.0(2) 27_565 15_444
Sr4B As1 Sr2A 81.0(2) 30 .
Sr4B As1 Sr2A 145.8(2) 30 15_444
Sr4B As1 Sr2B 155.0(4) 27_565 .
Sr4B As1 Sr2B 155.0(4) 30 15_444
Sr4B As1 Sr2B 88.3(3) 30 .
Sr4B As1 Sr2B 88.3(3) 27_565 15_444
Sr4B As1 Sr3 79.3(2) 30 25
Sr4B As1 Sr3 57.6(3) 27_565 25
Sr4B As1 Sr4A 16.0(3) 27_565 27_565
Sr4B As1 Sr4A 75.0(2) 30 27_565
Sr4B As1 Sr4A 75.0(2) 27_565 30
Sr4B As1 Sr4A 16.0(3) 30 30
Sr4B As1 Sr4B 72.0(4) 27_565 30
As4 As1 Sr1 61.33(4) . 8
As4 As1 Sr1 61.33(4) . 10_454
As4 As1 Sr2A 65.53(5) . .
As4 As1 Sr2A 65.53(5) . 15_444
As4 As1 Sr2B 57.1(3) . .
As4 As1 Sr2B 57.1(3) . 15_444
As4 As1 Sr3 116.51(4) . 25
As4 As1 Sr4A 138.91(4) . 30
As4 As1 Sr4A 138.91(4) . 27_565
As4 As1 Sr4B 144.0(2) . 27_565
As4 As1 Sr4B 144.0(2) . 30
Sr1 As2 Sr1 82.07(5) 8 4_554
Sr1 As2 Sr2B 75.8(3) 4_554 5
Sr1 As2 Sr2B 62.4(2) 4_554 14_554
Sr1 As2 Sr2B 125.9(3) 8 14_554
Sr1 As2 Sr2B 144.2(3) 8 5
Sr1 As2 Sr3 70.95(4) 8 27_565
Sr1 As2 Sr3 70.67(4) 4_554 27_565
Sr1 As2 Sr4A 137.26(6) 4_554 27_565
Sr1 As2 Sr4A 82.74(5) 8 27_565
Sr1 As2 Sr4B 78.3(2) 4_554 .
Sr1 As2 Sr4B 63.1(2) 8 .
Sr2A As2 Sr1 82.51(6) 5 4_554
Sr2A As2 Sr1 142.77(7) 5 8
Sr2A As2 Sr2B 8.8(2) 5 5
Sr2A As2 Sr2B 74.3(3) 5 14_554
Sr2A As2 Sr3 72.00(5) 5 27_565
Sr2A As2 Sr4A 144.08(7) 5 .
Sr2A As2 Sr4A 86.02(7) 5 27_565
Sr2A As2 Sr4B 144.47(18) 5 .
Sr2B As2 Sr2B 66.3(5) 5 14_554
Sr2B As2 Sr4A 94.8(3) 5 27_565
Sr2B As2 Sr4B 70.4(3) 14_554 .
Sr2B As2 Sr4B 136.1(3) 5 .
Sr3 As2 Sr2B 124.6(2) 27_565 14_554
Sr3 As2 Sr2B 75.3(3) 27_565 5
Sr3 As2 Sr4A 66.62(5) 27_565 27_565
Sr3 As2 Sr4B 127.2(2) 27_565 .
Sr4A As2 Sr1 69.53(5) . 8
Sr4A As2 Sr1 90.25(6) . 4_554
Sr4A As2 Sr2B 137.1(3) . 5
Sr4A As2 Sr2B 150.6(3) 27_565 14_554
Sr4A As2 Sr2B 71.3(3) . 14_554
Sr4A As2 Sr3 137.99(7) . 27_565
Sr4A As2 Sr4A 120.85(5) . 27_565
Sr4A As2 Sr4B 127.79(18) 27_565 .
Sr4A As2 Sr4B 13.0(2) . .
Zn1 As2 Sr1 135.38(6) 25 4_554
Zn1 As2 Sr1 135.59(6) 25 8
Zn1 As2 Sr2A 76.25(6) 25 5
Zn1 As2 Sr2B 74.2(2) 25 14_554
Zn1 As2 Sr2B 78.1(3) 25 5
Zn1 As2 Sr3 134.87(6) 25 27_565
Zn1 As2 Sr4A 80.12(5) 25 27_565
Zn1 As2 Sr4A 84.95(6) 25 .
Zn1 As2 Sr4B 97.1(2) 25 .
Zn2 As2 Sr1 129.3(4) 27_565 4_554
Zn2 As2 Sr1 121.5(5) 27_565 8
Zn2 As2 Sr1 133.1(5) . 4_554
Zn2 As2 Sr1 75.8(4) . 8
Zn2 As2 Sr2A 50.8(4) 27_565 5
Zn2 As2 Sr2A 136.7(5) . 5
Zn2 As2 Sr2B 59.2(5) 27_565 5
Zn2 As2 Sr2B 112.5(5) 27_565 14_554
Zn2 As2 Sr2B 99.2(5) . 14_554
Zn2 As2 Sr2B 139.2(5) . 5
Zn2 As2 Sr3 135.2(4) . 27_565
Zn2 As2 Sr3 76.2(4) 27_565 27_565
Zn2 As2 Sr4A 39.6(5) 27_565 27_565
Zn2 As2 Sr4A 43.4(5) . .
Zn2 As2 Sr4A 138.5(4) 27_565 .
Zn2 As2 Sr4A 80.2(5) . 27_565
Zn2 As2 Sr4B 54.9(5) . .
Zn2 As2 Sr4B 151.4(4) 27_565 .
Zn2 As2 Zn1 58.9(4) 27_565 25
Zn2 As2 Zn1 61.1(4) . 25
Zn2 As2 Zn2 97.4(5) . 27_565
Sr1 As3 Sr1 71.47(6) 8 .
Sr1 As3 Sr2A 158.52(7) 8 26_545
Sr1 As3 Sr4A 144.82(7) . 5
Sr1 As3 Sr4A 87.56(6) 8 5
Sr1 As3 Sr4A 67.89(6) . 8
Sr1 As3 Sr4A 111.08(7) 8 8
Sr1 As3 Sr4B 97.2(2) 8 8
Sr1 As3 Sr4B 63.36(19) . 8
Sr2A As3 Sr1 104.84(7) 26_545 .
Sr2A As3 Sr1 77.80(6) 10_454 .
Sr2A As3 Sr1 76.83(6) 10_454 8
Sr2A As3 Sr2A 81.71(7) 10_454 26_545
Sr2A As3 Sr4A 85.77(7) 26_545 8
Sr2A As3 Sr4A 138.90(7) 10_454 8
Sr2A As3 Sr4A 84.34(6) 26_545 5
Sr2A As3 Sr4A 69.93(7) 10_454 5
Sr2A As3 Sr4B 140.31(18) 10_454 8
Sr2A As3 Sr4B 99.8(2) 26_545 8
Sr2B As3 Sr1 70.5(3) 10_454 .
Sr2B As3 Sr1 69.0(3) 10_454 8
Sr2B As3 Sr2A 9.6(3) 10_454 10_454
Sr2B As3 Sr2A 89.7(3) 10_454 26_545
Sr2B As3 Sr3 148.9(3) 10_454 4_554
Sr2B As3 Sr4A 75.8(3) 10_454 5
Sr2B As3 Sr4A 135.3(3) 10_454 8
Sr2B As3 Sr4B 135.6(3) 10_454 .
Sr2B As3 Sr4B 133.8(3) 10_454 8
Sr3 As3 Sr1 123.81(7) 4_554 8
Sr3 As3 Sr1 138.48(6) 4_554 .
Sr3 As3 Sr2A 139.92(7) 4_554 10_454
Sr3 As3 Sr2A 73.45(6) 4_554 26_545
Sr3 As3 Sr4A 76.66(5) 4_554 5
Sr3 As3 Sr4A 70.63(5) 4_554 8
Sr3 As3 Sr4B 75.89(19) 4_554 8
Sr3 As3 Sr4B 59.4(2) 4_554 .
Sr4A As3 Sr4A 147.28(7) 8 5
Sr4A As3 Sr4B 14.1(2) 8 8
Sr4A As3 Sr4B 149.71(18) 5 8
Sr4B As3 Sr1 91.7(2) 5 8
Sr4B As3 Sr1 157.3(3) 5 .
Sr4B As3 Sr1 67.9(2) . 8
Sr4B As3 Sr1 104.9(2) . .
Sr4B As3 Sr2A 85.2(2) 5 26_545
Sr4B As3 Sr2A 83.7(3) 5 10_454
Sr4B As3 Sr2A 141.1(2) . 10_454
Sr4B As3 Sr2A 132.1(2) . 26_545
Sr4B As3 Sr2B 89.6(4) 5 10_454
Sr4B As3 Sr3 63.6(3) 5 4_554
Sr4B As3 Sr4A 13.9(3) 5 5
Sr4B As3 Sr4A 134.0(3) 5 8
Sr4B As3 Sr4A 92.2(2) . 5
Sr4B As3 Sr4A 71.96(19) . 8
Sr4B As3 Sr4B 81.5(4) 5 .
Sr4B As3 Sr4B 62.7(3) . 8
Sr4B As3 Sr4B 135.9(3) 5 8
Zn2 As3 Sr1 140.9(4) 8 8
Zn2 As3 Sr1 71.8(4) 8 .
Zn2 As3 Sr2A 107.8(4) 8 10_454
Zn2 As3 Sr2A 48.3(4) 8 26_545
Zn2 As3 Sr2B 110.1(5) 8 10_454
Zn2 As3 Sr3 78.2(4) 8 4_554
Zn2 As3 Sr4A 131.0(4) 8 5
Zn2 As3 Sr4A 40.7(4) 8 8
Zn2 As3 Sr4B 127.2(4) 8 5
Zn2 As3 Sr4B 109.8(5) 8 .
Zn2 As3 Sr4B 53.8(5) 8 8
Sr1 As4 Sr1 140.71(6) 10_454 .
Sr1 As4 Sr1 70.63(5) 10_454 15_444
Sr1 As4 Sr1 111.06(11) 15_444 .
Sr1 As4 Sr1 140.71(6) 8 15_444
Sr1 As4 Sr1 134.00(14) 10_454 8
Sr1 As4 Sr1 70.63(5) 8 .
Sr1 As4 Sr2A 82.33(7) 8 .
Sr1 As4 Sr2A 78.81(7) 10_454 .
Sr1 As4 Sr2A 82.33(7) 10_454 15_444
Sr1 As4 Sr2A 78.81(7) 8 15_444
Sr1 As4 Sr2B 69.2(3) 8 10_454
Sr1 As4 Sr2B 69.2(3) 10_454 8
Sr1 As4 Sr2B 143.2(3) 10_454 10_454
Sr1 As4 Sr2B 143.2(3) 8 8
Sr2A As4 Sr1 72.84(4) 15_444 .
Sr2A As4 Sr1 140.31(5) 15_444 15_444
Sr2A As4 Sr1 72.84(4) . 15_444
Sr2A As4 Sr1 140.31(5) . .
Sr2A As4 Sr2A 130.43(14) . 15_444
Sr2B As4 Sr1 87.1(3) 15_444 10_454
Sr2B As4 Sr1 75.8(3) 8 .
Sr2B As4 Sr1 68.4(3) 15_444 .
Sr2B As4 Sr1 66.4(3) 8 15_444
Sr2B As4 Sr1 142.9(3) . .
Sr2B As4 Sr1 66.4(3) 10_454 .
Sr2B As4 Sr1 87.1(3) . 8
Sr2B As4 Sr1 75.8(3) . 10_454
Sr2B As4 Sr1 75.8(3) 15_444 8
Sr2B As4 Sr1 68.4(3) . 15_444
Sr2B As4 Sr1 75.8(3) 10_454 15_444
Sr2B As4 Sr1 142.9(3) 15_444 15_444
Sr2B As4 Sr2A 77.2(3) 10_454 .
Sr2B As4 Sr2A 77.2(3) 8 15_444
Sr2B As4 Sr2A 134.4(3) 8 .
Sr2B As4 Sr2A 132.7(3) . 15_444
Sr2B As4 Sr2A 134.4(3) 10_454 15_444
Sr2B As4 Sr2A 4.8(3) . .
Sr2B As4 Sr2A 132.7(3) 15_444 .
Sr2B As4 Sr2A 4.8(3) 15_444 15_444
Sr2B As4 Sr2B 78.2(6) . 10_454
Sr2B As4 Sr2B 129.6(6) . 8
Sr2B As4 Sr2B 135.5(7) . 15_444
Sr2B As4 Sr2B 129.6(6) 15_444 10_454
Sr2B As4 Sr2B 110.5(6) 8 10_454
Sr2B As4 Sr2B 78.2(6) 15_444 8
As1 As4 Sr1 124.47(6) . 15_444
As1 As4 Sr1 67.00(7) . 8
As1 As4 Sr1 67.00(7) . 10_454
As1 As4 Sr1 124.47(6) . .
As1 As4 Sr2A 65.22(7) . 15_444
As1 As4 Sr2A 65.22(7) . .
As1 As4 Sr2B 124.8(3) . 8
As1 As4 Sr2B 124.8(3) . 10_454
As1 As4 Sr2B 67.7(3) . .
As1 As4 Sr2B 67.7(3) . 15_444
As4 As4 Sr1 113.00(7) 10_454 10_454
As4 As4 Sr1 55.53(6) 10_454 .
As4 As4 Sr1 55.53(6) 10_454 15_444
As4 As4 Sr1 113.00(7) 10_454 8
As4 As4 Sr2A 114.78(7) 10_454 15_444
As4 As4 Sr2A 114.78(7) 10_454 .
As4 As4 Sr2B 55.2(3) 10_454 10_454
As4 As4 Sr2B 112.3(3) 10_454 15_444
As4 As4 Sr2B 55.2(3) 10_454 8
As4 As4 Sr2B 112.3(3) 10_454 .
As4 As4 As1 180.0 10_454 .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Sr1 Sr2B 3.519(15) 15_444
Sr1 Sr2B 3.593(15) 10_454
Sr1 Sr4A 3.605(2) 8
Sr1 Sr4B 3.567(11) 8
Sr1 Zn2 3.511(19) 8
Sr1 As1 3.1989(19) 10_454
Sr1 As2 3.219(2) 8
Sr1 As2 3.242(2) 3_545
Sr1 As3 3.210(2) .
Sr1 As3 3.196(2) 8
Sr1 As4 3.404(3) .
Sr1 As4 3.049(2) 10_454
Sr2A Sr2B 0.547(13) .
Sr2A Sr3 3.758(2) 27_565
Sr2A Sr4A 3.720(3) 14_454
Sr2A Zn1 3.562(2) 29_554
Sr2A Zn2 2.466(19) 31_565
Sr2A As1 3.267(2) .
Sr2A As2 3.073(3) 5
Sr2A As2 3.619(3) 14_454
Sr2A As3 3.201(3) 26
Sr2A As3 3.188(3) 10_454
Sr2A As4 3.645(3) 10_454
Sr2A As4 3.275(3) .
Sr2B Sr2B 3.75(3) 10_454
Sr2B Zn2 2.98(2) 31_565
Sr2B As1 3.075(16) .
Sr2B As2 3.318(15) 5
Sr2B As2 3.537(16) 14_454
Sr2B As3 3.010(16) 10_454
Sr2B As3 3.660(14) 26
Sr2B As4 3.145(15) 10_454
Sr2B As4 2.791(15) .
Sr3 Sr4A 3.659(2) 6
Sr3 Sr4A 3.660(2) .
Sr3 Sr4B 3.106(14) 8
Sr3 Sr4B 3.106(14) 3_545
Sr3 Zn2 3.680(18) 6
Sr3 Zn2 3.680(18) .
Sr3 As1 3.4101(12) 20_656
Sr3 As1 3.4101(12) 25
Sr3 As2 3.312(2) 23_666
Sr3 As2 3.312(2) 20_656
Sr3 As3 3.080(2) 3_545
Sr3 As3 3.080(2) 8
Sr4A Sr4B 0.889(14) .
Sr4A Sr4B 3.779(12) 8
Sr4A Zn2 3.77(2) 20_656
Sr4A Zn2 2.14(2) .
Sr4A As1 3.204(3) 20_656
Sr4A As2 3.102(2) .
Sr4A As2 3.352(3) 20_656
Sr4A As3 3.301(3) 5
Sr4A As3 3.246(2) 8
Sr4B Sr4B 3.92(3) 5
Sr4B Sr4B 3.52(2) 8
Sr4B Zn2 2.94(3) .
Sr4B As1 2.995(11) 20_656
Sr4B As2 3.571(12) .
Sr4B As3 3.186(14) .
Sr4B As3 3.557(11) 8
Sr4B As3 2.799(11) 5
Zn1 Zn2 2.587(18) 25
Zn1 Zn2 2.587(18) 18_556
Zn1 Zn2 2.587(18) 12_454
Zn1 Zn2 2.587(18) 3_545
Zn1 As2 2.6746(16) 3_545
Zn1 As2 2.6746(16) 18_556
Zn1 As2 2.6746(16) 25
Zn1 As2 2.6746(16) 12_454
Zn2 As2 2.582(19) 20_656
Zn2 As2 2.396(17) .
Zn2 As3 2.739(17) 8
As1 As4 2.726(4) .
As4 As4 0.735(7) 10_454
